Int. J. Chem. Sci, Volume: 15( 4)
Structural and Surface Roughness Effects on Sensing Properties of Zno Doping with Al Thin Films Deposited by Spray Pyrolysis Technique
- Mohammed MA University of Al-Qadisiyah, College of Agriculture, Iraq, Tel: +964-780978 2478; E-mail: [email protected]
Received Date: October 07, 2017 Accepted Date: October 27, 2017 Published Date: October 31, 2017
Citation: Salman SR, Mohammed MA. Structural and Surfac? Roughn?ss Effects on S?nsing Properti?s of ZnO Doping with Al Thin Films D?posited by Spray Pyrolysis T?chnique. Int J Chem Sci. 2017;15(4):211
In this article, the gÐ°s sensor properties of ZnO doping with (2% and 4% wt.) Al thin films hÐ°ve beÐµn accounted for, where the nanocrystÐ°lline ZnO based thin films wÐµre all around kept by Ð° straight forward and chemicÐ°l sprÐ°y pyrolysis (CSP) system. Films have been observed to be uniform, pinhole free and wÐµll disciple to the substrate. The morphology, structures and surface harshness of the stored Al doped ZnO thin films were contemplated by different sorts of portrayal strategies. The creators have watched that the sÐµnsor reaction and selÐµctivity towards CO gas is enhanced by the Al doping at a low temperaturÐµ. XRD showÐµd the acquired films are nanocrystalline in naturÐµ with hexagonal wurtzite phase. The films were utilized for identification of CO noticeable all around and most extreme reaction was seen at 175°C. The change in sÐµnsor rÐµsponse of ZnO:Al thin films to CO gÐ°s credited to thÐµ imperfection chemistry, crystallite size and surface roughnÐµss.
ZnO: Al; Gas sensor; Thin films; Chemical spray pyrolysis
Metal oxides (MOs) have picked up an impressive research enthusiasm because of its minimal effort and straightforward handling steps and high potential for the electronic and optoelectronic applications [1-4]. The advance in the field of using MOs for gas detecting application was highlighted by the high detecting capacities of MOs and their physical properties, for example, electrical transport, attractive, optical reaction, warm conductivity and superconductivity [5-9]. The MOs semiconductor materials have been broadly examined in gas detecting applications because of their simplicity of recognition both oxidizing and decreasing gasses. Among different MOs semiconductors, ZnO is an immediate, wide band crevice (Eg=3.37 eV at room temperature) and most encouraging multifunctional material in view of its plenitude in nature, more affordable and has high exciton restricting vitality of 60 meV, which makes the exciton state stable even at room temperature [10,11]. Moreover, its biodegradable and biocompatible properties likewise make it a reasonable contender for different applications [12-20].
ZnO based electronic gadgets, for example, gas sensors are anticipated to be a superior worker and empower the new capacities . Besides, the streamlined doped ZnO thin film has a tremendous potential for understanding the detecting properties and their working component. Be that as it may, the negative and less uncovered surface territory of ZnO nanostructure ought to be controlled amid the amalgamation procedure to improve the detecting capacity. In this way, to blend and investigate the detecting conduct of the doped ZnO nanostructure and to additionally comprehend the bits of knowledge of detecting component is one of the points of the present reviews.
The doped and un-doped nanostructures of the ZnO thin films have been orchestrated with using a few techniques, for example, sputtering , sol gel  and spin coating  etc. The basic element between the said procedures is the necessity of complex and controlled condition that prompts an expansion in cost and intricacies all the while. Be that as it may, a non-vacuum based (CSP) prepare, a non-vacuum process, is more helpful, alongside minimum costly and reasonable for substantial territory of affidavit .
One of the upsides of this procedure in regard to doping of tests is that it is anything but difficult to dope the specimens of any component whose salt can be disintegrated in the shower arrangement. The developing worldwide worries for ecological security, contamination and its impacts have invigorated the consideration of the exploration group in the creating field of gas sensor. CO is generally created in transportations and mechanical apparatuses and it is perilous in nature and its spillage recognition is likewise a critical issue. The uses of the MOs for gas detecting has been generally considered. In any case, the testimony of nanocrystalline thin films of Al-doped ZnO and their morphological and basic impact on gas detecting properties are once in a while found in the writing.
In the present review, we r?port the amalgamation of ZnO and Al-dop?d ZnO bas?d thin films by a basic and cheap strategy, i.e., CSP and it is described to assess its gas detecting prop?rties. Structur? and surfac? morphology of the films were researched by (XRD), (AFM) and scanning electron microscopy (SEM). The sensor reactions of unadulterated and Al-dop?d ZnO movies were contemplated for CO gas. The impact of working temperature on sensor response of kept films towards CO introduction is discussed.
Pure and dop?d ZnO:Al films on a glass substrate were deposited by CSP technique. Zn(CH3COO)2.2H2O and AlCl3·6H2O was utilized as source materials for the testimony of thin films. Glass substrates were cleaned with water, then washed with ethanol, then using ultrasonic cleaner. 0.1 M forerunners were dissolved in ethanol. Al doping concentration changed from 2 to 4 wt%. The mixing was utilizing using an ultra-sonication for 20 min. The resulting solution was sprayed onto the glass substrate by atomizer. The deposition temperature was maintained at 40°C. The distance between the substrate and atomizer was 30 cm.
X-ray diffraction investigation was utilized to perceive the precious stone structure of ZnO pure and doped films using X-ray diffraction instrument type (Shimadzu 6000) with wavelength of 1.5045 ? and the scanning range 20°-80°. Surface topography of these films was studied by atomic force microscopy (AFM) using a Digital Instruments, Inc. BY3000. The morphology of thin films was examining by scanning electron microscopy (SEM) type Inspect 550. Gas sensing experiments were performed with were measured by using homemade equipment at an operating temperature 100 to 300°C.
Results and Discussion
Figure 1 portrays the XRD of ZnO pure and doped thin films. The got diffraction of tests films are hexagonal crystal structure of ZnO (JCPDS card document 36-1451). From the indicated XRD design in Figure 1, it is watched that intensity of the peak decreases with Al fuse in ZnO lattice and width has turned out to be more extensive approving little grain formation. Closely, this behavior has been earlier reported by Kim et al. .
The crystallite sizes (D) of the ZnO:Al thin films was employed by using Scherer’s formula and is given by:
Where k equal 0.94 (constant), λ is wavelength of the X-Ray equal 1.54?, β is the full width at half maxima (FWHM) (in radians) of the diffraction peak. The average crystallite size of films was found in Table 1. Note that the average of grain size decreases with increasing Al wt%, this shows a development in the structural properties of the films.
Table 1. XRD parameters for ZnO:Al thin films.
Additionally, for more information on the amount of defects in the thin films, the number of layers (Nl), micro strain (ε), dislocation density (δ), specific surface area (SSA)  and texture coefficient Tc(hkl)  were evaluated as shown in Table 2 from equations (2-6) respectively.
|Sample||Average Nl × 1017 (m-2)||Average ε%||Average δ × 1016 (m-2)||SSA
Table 2. Number of layers (Nl), micro strain (ε), dislocation density (δ), specific surface area (SSA) and texture coefficient Tc(hkl) for ZnO:Al thin films.
Where ρ is bulk density for ZnO equal 0.88 gm/cm3.
Where, Tc(hkl) is the texture coefficient of the hkl plane, I(hkl) is the measured intensity, Io(hkl) is the relative intensity of the corresponding plane given in PDF-2 data and N is the number of reflections.
From Table 2, The variation of layer number varies with pure and doped thin films in a random way. It is thought that the quantity of drop plays a great role in this random change. The micro strain depends directly on the lattice constant (c) and its value related to the shift from the JCPDS file no. 36-1451 value. The values of micro strain increase with increasing Al wt% in the films. The dislocation density is the measure of amount of defects in a crystal. Note the value of average dislocation density obtained in the present work decreases with increase of Al wt%.
This confirmed good crystallinity of prepared thin films. Also, From Table 2, show increase Specific surface area and texture coefficient with increase of Al wt%. The surface of the synthesized materials is found to be very large and hence the heterogeneous catalytic property of the material were tested and found positive response.
The standard information for d-separating estimations of ZnO wer? tak?n from JCPDS r?cord no. 36-1451. It is watched that with an expansion in aluminum convergence of the films, scattered-ness of Δd/d values incr?ase. It derives the presentation of stacking shortcomings with the joining of various grouping of aluminum in ZnO films. Subjectively, the scattered-ness of Δd/d values show the thickness of stacking issues exhibit in the films . It can, in this way, be construed that aluminum joining prompts an expansion in the stacking issue thickness of the ZnO thin films with an incr?ase in the lattice param?ter.
Th? morphology and microstructur? of the surface of the ZnO:Al thin films were examined by the AFM. The ZnO:Al films are appeared in Figure 3. The surface morphologies for various doping centralizations of the films appear to be dense; the topography pictures nearly don't show any changes and make known good quality films. The smooth surface was plainly observed for ZnO pure, an increasing in Al add up to ZnO lattice appeared with a high surface roughness. The 4 wt% Al doped ZnO thin films, showed that the littler particles agglomerated and made bigger globules particles as compares to another. Subsequently, these results favor the shape distortion of crystallites in Al doped ZnO thin films ascribed to all the more stacking defects display in the films. The root mean squares (RMS) roughness of thin films with 0%, 2% and 4% Al are 14 nm, 17 nm and 20 nm. These results are like different reports [29,30].
Figure 4 appear the SEM image of the ZnO:Al thin. The micrograph obviously modulation in the averag? grain siz? with an increas? in Al wt%. Figure 4 demonstrates that the thin films ar? uniform and grains ar? around circular in nature. Both the XRD image and the SEM micrographs infer that the expansion of Al in ZnO grid confines the development of grains. The normal grain measure seen if there should be an occurrence of the immaculate ZnO film was around 95 nm and found to diminish ~40 and ~23 nm for 2 and 4 wt% Al.
The evaluated crystallite sizes utilizing Scherer's equation and from SEM micrographs for ZnO:Al films are not comparable with each other, it might be expected to the presence of indistinct stage around the grains.
Figure 5. Shows sensor response with CO concentration, it has been watched that the 4 wt% Z nO:Al sensor showed the most extreme affectability to CO when contrasted with another. The sensor reaction increments with CO concentration up to 100 ppm and sensor reaction immersed past 100 ppm of CO gas presentation. The immersion in the sensor reaction past 100 ppm of CO gas credited to constrained response destinations existing on the film surface. The temperature-subordinate sensor reaction of Al doped ZnO thin films was contemplated in the temperature scope of 100°C to 300°C to discover the ideal working temperature for CO sensing.
Figure 6 explain the sensor reactions as a function of temperature. The sensor response of 4 wt% Al is phenomenal at 175°C, though ZnO thin films demonstrated sensor response at higher working temperature ~275°C. The sensitivity conducts of thin films have been considered for various concoction inputs.
In conclusion, we examined the effect of crystallite size, stacking deformity and higher surface roughness on the sensor response of ZnO doped with Al by using CSP. The CSP method has given pinhole free thin films with a uniform dispersion of grains and well disciple nanocrystalline ZnO based thin films. Deposited films have affirmed the polycrystalline nature with wurtzite hexagonal structure and favored introduction along (002) plane. AFM and SEM showed spherical growth of ZnO:Al grains. The 4 wt% Al doped ZnO sensor shows high response to CO. Best outcomes were achieved in 4 wt% Al doped ZnO sensor at 175°C. The extensive surface area, higher surface roughness and all the more stacking deformities are in charge of upgraded sensor response to CO gas.
- Huang JH, Huang TY, Wei HY, et al. Wet-milled transition metal oxide nanoparticles as buffer layers for bulk heterojunction solar cells. RSC Adv. 2012;2:7487-91.
- Vasilopoulou M, Palilis LC, Georgiadou DG, et al. Tungsten oxides as interfacial layers for improved performance in hybrid optoelectronic devices. Thin Solid Films. 2011;519:5748-53.
- Hasan NB, Mohammed MA. Optical characterization of (PbO)1-x (CdO)x deposited by spray pyrolysis technique. J Elec Dev. 2015;22:1924-9.
- Fan F, Feng Y, Bai S, et al. Synthesis and gas sensing properties to NO2 of ZnO nanoparticles. Sens Actuat B-Chem. 2013;185:377-82.
- Masuda Y, Itoh T, Shin W, et al. SnO2 nanosheet/nanoparticle detector for the sensing of 1-nonanal gas produced by Lung Cancer. Sci Rep. 2015;5:10122.
- Gasperaa ED, Guglielmia M, Martuccia A, et al. Enhanced optical and electrical gas sensing response of sol-gel based NiO-Au and ZnO-Au nanostructured thin films. Sens Actuat. 2012;164:54-63.
- Diyatmika W, Chu JP, Kacha BT, et al. Thin film metallic glasses in optoelectronic, magnetic and electronic applications: A recent update. Curr Opin Solid State Mater Sci. 2015;19:95-106.
- Cao J, Wu J. Strain effects in low-dimensional transition metal oxides. Materials Science and Engineering: R: Reports 2011;71:35-52.
- He Z, Wang X. Renewable energy and fuel production over transition metal oxides: The role of oxygen defects and acidity. Catal Today. 2015;240:220-8.
- Willander M, Israr MQ, Sadaf JR, et al. Progress on one-dimensional zinc oxide nanomaterials based photonic devices. Nanophotonics. 2012;1:99-115.
- Benharrats F, Zitouni K, Kadri A, et al. Determination of piezoelectric and spontaneous polarization fields in quantum wells grown along the polar <0001> direction. Superlattices Microstruct. 2010;47:592-6.
- Huang J, Yin Z, Zheng Q. Applications of ZnO in organic and hybrid solar cells. Energy Environ Sci. 2011;4:3861-77.
- Djurisic AB, Chen X, Leung YH, et al. ZnO nanostructures: Growth, properties and applications. J Mater Chem. 2012;22:6526-35.
- Li S, Sun Z, Li R, et al. ZnO nanocomposites modified by hydrophobic and hydrophilic silanes with dramatically enhanced tunable fluorescence and aqueous ultra-stability toward biological imaging applications. Sci Rep. 2015;5:8475.
- Hameed ASH, Karthikeyan C, Ahamed AP, et al. In-vitro antibacterial activity of ZnO and Nd doped ZnO nanoparticles against ESBL producing Escherichia coli and Klebsiella pneumonia. Sci Rep. 2016;6:24312.
- Tang X, Choo ESG, Li L, et al. Synthesis of ZnO nanoparticles with tunable emission colors and their cell labeling applications. Chem Mater. 2010;22:3383-8.
- Lin WH, Chang TFM, Lu YH, et al. Supercritical CO2-assisted electrochemical deposition of ZnO mesocrystals for practical photo-electro-chemical applications. J Phys Chem. 2013;117:25596-60.
- Wang J, Lee YJ, Hsu JWP. One-step synthesis of ZnO nanocrystals in n-butanol with band-gap control: Applications in hybrid and organic photovoltaic devices. J Phys Chem. 2014;pp:18417-23.
- Chen D, Zhao Y, Chen Y, et al. One-step chemical synthesis of ZnO/graphene oxide molecular hybrids for high-temperature thermoelectric applications. ACS Appl Mater Interfaces. 2015;7:3224-30.
- Li Z, Yang R, Yu M, et al. Cellular level biocompatibility and biosafety of ZnO nanowires. J Phys Chem. 2008;112:20114-7.
- Zhang J, Liu X, Neri G, et al. Nanostructured materials for room-temperature gas sensor. Adv Mater. 2016;28:795-831.
- Yang PF, Wen HC, Jian SR, et al. Characteristics of ZnO thin films prepared by radio frequency magnetron sputtering. Microelectron Reliab. 2008;48:389-94.
- Tsay CY, Hsu WT. Sol-gel derived undoped and boron-doped ZnO semiconductor thin films: Preparation and characterization. Ceram Int. 2013;39:7425-32.
- Poongodi G, Kumar RM, Jayavel R. Structural, optical and visible light photocatalytic properties of nanocrystalline Nd doped ZnO thin films prepared by spin coating method. Ceram Int. 2015;41:4169-75.
- Kumar M, Kumar A, Abhyankar AC. SnO2 based sensors with improved sensitivity and response recovery time. Ceram Int. 2014;40:8411-8.
- Kim H, Pique A, Horwitz JS, et al. Effect of aluminum doping on zinc oxide thin films grown by pulsed laser deposition for organic light-emitting devices. Thin Solid Films. 2000;377:798-802.
- Mandal D, Bolander ME, Mukhopadhyay D, et al. The use of microorganisms for the formation of metal nanoparticles and their application. Appl Microbiol Biotechnol. 2006;69:485-92.
- Nasser SA, Afify HH, E-Hakim SA, et al. Structural and physical properties of sprayed copper–zinc oxide films. Thin Solid Films. 1998;315:327.
- Kaur J, Roy SC, Bhatnagar MC. Highly sensitive SnO2 thin film NO2 gas sensor operating at low temperature. Sens Actuators. 2007;123:1090-95.
- Mende LS, Driscoll JLM. ZnO-nanostructures, defects and devices. Mater Today. 2007;10:40-8.